Towards fast femtosecond laser micromachining of fused...
Embed Size (px)
Transcript of Towards fast femtosecond laser micromachining of fused...
Towards fast femtosecond laser micromachining
of fused silica: The effect of deposited energy.
Sheeba Rajesh and Yves Bellouard
Micro- & Nano- Scale Engineering, Mechanical Engineering Department, Eindhoven University of Technology, P.O.
Box 513, 5600 MB, Eindhoven, The Netherlands.
Abstract: Femtosecond laser micromachining of glass material using low-
energy, sub-ablation threshold pulses find numerous applications in the
fields of integrated optics, lab-on-a-chips and microsystems in general. In
this paper, we study the influence of the laser-deposited energy on the
performance of the micromachining process. In particular, we show that the
energy deposited in the substrate affects its etching rate. Furthermore, we
demonstrate the existence of an optimal energy deposition value. These
results are not only important from an industrial point-of-view but also
provide new evidences supporting the essential role of densification and
consequently stress-generation as the main driving factor promoting
enhanced etching rate following laser exposure.
©2010 Optical Society of America
OCIS codes: (140.7090) Ultrafast lasers; (160.2750) Glass and other amorphous materials;
(320.2250) femtosecond phenomena; (320.7130) Ultrafast processes in condensed matter,
References and links
1. K. M. Davis, K. Miura, N. Sugimoto, and K. Hirao, “Writing waveguides in glass with a femtosecond laser,”
Opt. Lett. 21(21), 1729–1731 (1996).
2. Y. Sikorski, A. Said, P. Bado, R. Maynard, C. Florea, and K. Winick, “Optical waveguide amplifier in Nd-doped
glass written with near-IR femtosecond laser pulses,” Electron. Lett. 36(3), 226–227 (2000).
3. K. Minoshima, A. M. Kowalevicz, I. Hartl, E. P. Ippen, and J. G. Fujimoto, “Photonic device fabrication in glass
by use of nonlinear materials processing with a femtosecond laser oscillator,” Opt. Lett. 26(19), 1516–1518
4. S. Nolte, M. Will, J. Burghoff, and A. Tuennermann, “Femtosecond waveguide writing: a new avenue to three-
dimensional integrated optics,” Appl. Phys., A Mater. Sci. Process. 77(1), 109–111 (2003).
5. R. Osellame, S. Taccheo, M. Marangoni, R. Ramponi, P. Laporta, D. Polli, S. De Silvestri, and G. Cerullo,
“Femtosecond writing of active optical waveguides with astigmatically shaped beams,” J. Opt. Soc. Am. B
20(7), 1559–1567 (2003).
6. R. W. A. Applegate, Jr., J. Squier, T. Vestad, J. Oakey, D. W. M. Marr, P. Bado, M. A. Dugan, and A. A. Said,
“Microfluidic sorting system based on optical waveguide integration and diode laser bar trapping,” Lab Chip
6(3), 422–426 (2006).
7. Y. Hanada, K. Sugioka, H. Kawano, I. S. Ishikawa, A. Miyawaki, and K. Midorikawa, “Nano-aquarium for
dynamic observation of living cells fabricated by femtosecond laser direct writing of photostructurable glass,”
Biomed. Microdevices 10(3), 403–410 (2008).
8. Y. Bellouard, A. Said, and P. Bado, “Integrating optics and micro-mechanics in a single substrate: a step toward
monolithic integration in fused silica,” Opt. Express 13(17), 6635–6644 (2005),
9. Y. Bellouard, A. Said, M. Dugan, and P. Bado, “Monolithic integration in fused silica: When fluidics, mechanics
and optics meet in a single substrate,” in International Symposium on Optomechatronic Technologies (2009), pp.
10. A. Marcinkevi Ius, S. Juodkazis, M. Watanabe, M. Miwa, S. Matsuo, H. Misawa, and J. Nishii, “Femtosecond
laser-assisted three-dimensional microfabrication in silica,” Opt. Lett. 26(5), 277–279 (2001).
11. Y. Bellouard, A. Said, M. Dugan, and P. Bado, “Fabrication of high-aspect ratio, micro-fluidic channels and
tunnels using femtosecond laser pulses and chemical etching,” Opt. Express 12(10), 2120–2129 (2004),
12. S. Kiyama, S. Matsuo, S. Hashimoto, and Y. Morihira, “Examination of Etching Agent and Etching Mechanism
on Femotosecond Laser Microfabrication of Channels Inside Vitreous Silica Substrates,” J. Phys. Chem. C
113(27), 11560–11566 (2009).
#133139 - $15.00 USD Received 10 Aug 2010; revised 5 Sep 2010; accepted 8 Sep 2010; published 24 Sep 2010 (C) 2010 OSA 27 September 2010 / Vol. 18, No. 20 / OPTICS EXPRESS 21490
13. C. Hnatovsky, R. S. Taylor, E. Simova, V. R. Bhardwaj, D. M. Rayner, and P. B. Corkum, “Polarization-
selective etching in femtosecond laser-assisted microfluidic channel fabrication in fused silica,” Opt. Lett.
30(14), 1867–1869 (2005).
14. C. Schaffer, J. García, and E. Mazur, “Bulk heating of transparent materials using a high-repetition-rate
femtosecond laser,” Appl. Phys., A Mater. Sci. Process. 76(3), 351–354 (2003).
15. S. Eaton, H. Zhang, P. Herman, F. Yoshino, L. Shah, J. Bovatsek, and A. Arai, “Heat accumulation effects in
femtosecond laser-written waveguides with variable repetition rate,” Opt. Express 13(12), 4708–4716 (2005),
16. W. Yang, P. G. Kazansky, Y. Shimotsuma, M. Sakakura, K. Miura, and K. Hirao, “Ultrashort-pulse laser
calligraphy,” Appl. Phys. Lett. 93(17), 171109 (2008).
17. W. Yang, P. G. Kazansky, and Y. P. Svirko, “Non-reciprocal ultrafast laser writing,” Nat. Photonics 2(2), 99–
18. B. Poumellec, M. Lancry, J.-C. Poulin, and S. Ani-Joseph, “Non reciprocal writing and chirality in femtosecond
laser irradiated silica,” Opt. Express 16(22), 18354–18361 (2008),
19. J. W. Chan, T. Huser, S. Risbud, and D. M. Krol, “Structural changes in fused silica after exposure to focused
femtosecond laser pulses,” Opt. Lett. 26(21), 1726–1728 (2001).
20. Y. Bellouard, E. Barthel, A. A. Said, M. Dugan, and P. Bado, “Scanning thermal microscopy and Raman
analysis of bulk fused silica exposed to low-energy femtosecond laser pulses,” Opt. Express 16(24), 19520–
19534 (2008), http://www.opticsinfobase.org/oe/abstract.cfm?URI=oe-16-24-19520.
21. Y. Bellouard, T. Colomb, C. Depeursinge, M. Dugan, A. A. Said, and P. Bado, “Nanoindentation and
birefringence measurements on fused silica specimen exposed to low-energy femtosecond pulses,” Opt. Express
14(18), 8360–8366 (2006), http://www.opticsinfobase.org/oe/abstract.cfm?URI=oe-14-18-8360.
22. M. Tomozawa, Y. Lee, and Y. Peng, “Effect of uniaxial stresses on silica glass structure investigated by IR
spectroscopy,” J. Non-Cryst. Solids 242(2-3), 104–109 (1998).
23. A. Agarwal, and M. Tomozawa, “Correlation of silica glass properties with the infrared spectra,” J. Non-Cryst.
Solids 209(1-2), 166–174 (1997).
24. Y. Shimotsuma, P. G. Kazansky, J. Qiu, and K. Hirao, “Self-organized nanogratings in glass irradiated by
ultrashort light pulses,” Phys. Rev. Lett. 91(24), 247405 (2003).
25. K. Awazu, and H. Kawazoe, “Strained Si–O–Si bonds in amorphous SiO2 materials: A family member of active
centers in radio, photo, and chemical responses,” J. Appl. Phys. 94(10), 6243–6262 (2003).
1. Introduction: femtosecond laser process combined with chemical etching
Femtosecond laser processing with low-energy pulses eventually combined with chemical
etching of dielectrics is finding numerous promising applications not only for integrated
optics (see for instance [1–5]) but also for lab-on-a-chip (see for instance [6,7]) and more
generally for highly integrated three-dimensional monolithic microsystems  that combine
optical, fluid-handling and mechanical functions in a single substrate . Although various
substrates have been considered (for instance photo-etchable glass ), fused silica (the
glassy phase of SiO2) offers the most attractive properties such as low self-fluorescence, high
chemical stability and a broad transmission spectrum.
The process of femtosecond laser exposure combined with etching - first reported by
Markincevicius et al.  for fused silica - involves two steps that are depicted in Fig. 1.
First, the substrate is exposed to a tightly focused femtosecond laser-beam emitting low-
energy pulses, typically below or in the range of 1µJ. Patterns are ‘written’ by moving the
specimen under the laser beam (for instance using motorized stages). The pulse energy levels
are such that no material is removed but structural modifications of the material take place at
the laser focal spot. The process for making any arbitrary shape is further described in .
#133139 - $15.00 USD Received 10 Aug 2010; revised 5 Sep 2010; accepted 8 Sep 2010; published 24 Sep 2010 (C) 2010 OSA 27 September 2010 / Vol. 18, No. 20 / OPTICS EXPRESS 21491
Step 1: Laser exposure (no ablation) Step 2: Chemical etching
Laser exposed patterns Glass substrate
Fig. 1. Illustration of the femtosecond laser processing combined with chemical etching. In a
first step, the material is expose